FSC 7530 JCP F30
25% GLAZED MANIFOLD
Manifold Paper February 1, 1999
Use information: This paragraph is informational only and is not exclusively definitive of the end use.
For offset printing, generally face only, of multiforms and for multiple copies of correspondence, requiring above average permanence.
Light weight, low bulk, and low opacity. Printed matter may include text and light line illustrations.
Stock: Not less than 25 pct cotton or linen fibers. Groundwood General appearance: Paper shall conform to the standard sam-
pulp, not to exceed 1 pct. ple(s) adopted by the Government.
Note: 1 Postconsumer recovered fiber, in any percentage, is en- Color: The paper in the order (or publication) shall be uniform
couraged, provided that the requirements of this Standard are
met. with a target brightness of 80 pct. The color variation shall not
Acidity: pH value shall average not less than 6.5.
Finish and formation: Shall be uniform.
Grammage (g/m 2) .............................................................. 30
Basis weight: 17 by 22 inches, 500 sheets (pounds) ...... 8 Cleanliness: The dirt count for each side of the paper shall not
A tolerance of ±5 pct shall be allowed. exceed 250 specks per square meter. No sample sheet (600 to
650 cm2 in size) shall contain more than one defect with an
Bursting strength: Average, not less than (kPa) ........... 60
Equivalent (lb/in 2) ........................................................... 10 equivalent area of 0.25 mm2 or greater.
Writing quality: Characters written with ball point and felt tip Sampling and testing: Shall be conducted in accordance with
pens shall be clear cut and free from excessive feathering. standards in Part 2, Government Paper Specification Standards.
Unless otherwise specified, the following is automatically waived when printing or duplicating is to be accomplished on commercial contract
Sizing: Paper shall be surface- and internal-sized suitable for sat- smooth edges, and evenly jogged. A tolerance of ±2 mm (1⁄16
isfactory printing on both sides of the paper on high-speed offset inch) shall be allowed except for sheets 216 by 356 mm (81⁄2 by
presses equipped with continuous flow or brush dampening sys- 14 inches) or less; then a tolerance of ±1 mm (1⁄32 inch) shall be
tems. allowed. Successive sheets within any package shall not differ
Color: Shall match the Government’s standard sample for color. from each other by more than 0.5 mm (1⁄64 inch). Paper with the
A deviation of DE(CIELAB)±3.0 from the color standard is al- long dimension 813 mm (32 inches) or less shall be considered
lowed. square if the variation does not exceed 1 mm (1⁄32 inch); over
813 mm (32 inches), 2 mm (1⁄16 inch).
Curl: Paper shall lie flat with either no tendency to curl or with
a curl which can be overcome under reasonable working condi- Grain: Direction of the grain on flat paper shall be as ordered.
tions. Pressroom conditions: The bulk of this paper will be used in
Size and trim: Sheets: Paper shall be furnished in the size(s) or- air-conditioned pressrooms maintained at 24 °C ±2 °C and 45 pct
dered and shall be flat, trimmed square on four sides with clean ±8 pct relative humidity.
1 This grade is typically a low Government usage paper and currently not readily and/or economically available with postconsumer
recovered fiber content. If a postconsumer fiber content is desired in the paper, that number will be stated in the procurement document.
Note, recovered material (cotton/linen) is not a postconsumer recovered fiber.